CHAPTER 4: RESULTS AND DISCUSSION
4.2.1. The Bragg –Williams LRO parameter
Precise value of the long – range order parameter have been determined in a large number of A15 type compounds, as for example Nb3Ir, Nb3Pt  or Nb3Al . The case of Nb3Sn is particular: due to the small difference between the form factors of Nb and Sn (fNb and fSn) which is a consequence of the proximity of Nb and Sn in the periodic system (∆𝑍𝑍 = 9). The relative intensity of the superlattice reflection (110) is quite low, resulting in a ratio I(110)/I(211) as low as 0.14 for perfect ordering. This low ratio in the relative intensity of the superlattice reflections for Nb3Sn compound increases the uncertainty ∆𝑆𝑆. It follows that the determination of a precise order parameter for Nb3Sn requires not only homogeneous and very well defined samples, but also an excellent X – ray counting statistics, the error reaching ±0.04 in low quality Nb3Sn samples. Sweedler et al.  reported perfect ordering of S=1 for Nb3Sn before irradiation (corresponding to the very low electrical resistivity), but gave no details of the diffraction data were given, neither about the line intensities nor about the refinement procedure. Other authors 156][155, 156] studying irradiation effects on Nb3Sn assumed perfect ordering, too, based on the data of Sweedler et al. .
The present work thus constitutes the first complete Rietveld refinement of the Bragg – Williams long – range order parameter in Nb3Sn by means of X – ray diffractometry data.
Rietveld Refinement (Full Prof software) before proton irradiation
As previously reported (Subsection 2.2.4), the Bragg-Williams long range order parameter before irradiation (Nb3Sn sample #4) S = Sa = Sb = 0,98 ± 0,02 was estimated through the Rietveld Refinement procedure (described in Section 3.3) and it is an average values obtained after a dozen of X – ray measurements performed on the same sample.
This value corresponds to a state of atomic ordering very close to perfect ordering: Sa is associated to an occupation factor of Nb in 6c sites of ra = 0,997±0,003 and Sb is associated to an occupation factor of Sn in 2a sites of rb = 0,991±0,003.
This result justifies a posteriori the value assumed by Sweedler et al. : S=1 on Nb3Sn before irradiation.
From a least-square fit, the lattice constant, a, and the isotropic temperature factor, Biso, were found to be 5,291±0,003 Å and 0,407±0,003 Å respectively. These experimental values are in good agreement with the theoretical one: Bthiso = 0.4 Å estimated in Subsection 1.2.2 and a=5,289±0.01 Å found by Devantay at al.  for Nb3Sn at the stoichiometric composition (25 at.%Sn).
The agreement factors for the Rietveld refinement performed in the present work are reported in Table 10. The excellent values for these factors ensure the goodness of the refinement procedure and thus of the results.
Agreement Factor Value Expected limit
Rexp 6.46 <15
GofF 1.59 <2
χ2 2.5 ~1
Table 10 Agreement Factors. The slightly higher value for the χ2 has to be assigned to the preferential orientation that was not taken into account during the refinement procedure due to the high number of parameters in the model (see Subsection 3.3.1).
In order to exclude the influence of texture effects, the Bragg Williams LRO parameter has also been estimated with the simple method described in Subsection 3.3.1 (See “Empirical method to extrapolate the S value”). By means of such extrapolation, averaging on the peaks (110), (211), (222), (320), (321), (400), (332) and (440), it was found that Sempirical = 0.979, i.e. it is in perfect agreement with the refined value.
Synchrotron analysis after proton irradiation
To investigate the effects at the Bragg peak (see Subsection 3.1.2) on the microscopic structure and thus, to get some information on the variation of the lattice constant, of the microstrain and
of the Bragg Williams LRO parameter, a set of three pairs of Nb3Sn platelets have been irradiated with 10 MeV protons at the Kurchatov’s cyclotron U-150 at different fluences:
- Platelets with thicknesses of 0.18 (steady loss) and 0.12 mm (Bragg peak) irradiated at a fluence of 3 × 1020 p/m2;
- Platelets with thicknesses of 0.20 (steady loss) and 0.18 mm (Bragg peak) irradiated at a fluence of 3 × 1021 p/m2;
- Platelets with thicknesses of 0.20 (steady loss) and 0.18 mm (Bragg peak) irradiated at a fluence of 1 × 1022p/m2;
- Pristine platelet with thickness of 0.18 mm has been measured for consistency of the results (see later on).
In the following the sample in the steady loss and in the Bragg peak regions will be indicated as
#1 and #2 respectively. The description of the general arrangement of the Nb3Sn platelets with respect to the proton beam has already described in Subsection 3.1.2. Due to the lack of the important information about the distribution of the energy deposition inside the two samples (-dE/dx) from which it would have been possible to estimate the exact position of the Bragg peak inside samples #2 we tried to figure out where the Bragg peak should be located taking into account from FLUKA simulation the dpa vs the proton penetration depth and the thickness of the two samples sent to the Kurchatov Institute. Thus, in Figure 70 the estimated position of the two platelets (#1 and #2) with respect to the stopping power at 10 MeV for each proton fluence is shown.
Figure 70 Description of the approximate position of the two platelets (#1 and #2) with respect to the stopping power calculated by means of FLUKA simulation for each proton fluence.
Due to safety prescription due to radioactivity, it was not possible to perform X-ray diffraction measurements at the University of Geneva: the irradiated samples were thus studied at the Kurchatov Institute by means of synchrotron X-ray powder diffraction (XRPD) and resonant diffraction (REXD) by Y. Zubavichus. As will be explained hereafter, resonant diffraction measurements (also known as Anomalous X-ray scattering) have the advantage to overcome the problems due to the texture effects in the determination of the Bragg Williams LRO parameter.
According to the refinement procedure performed by Y. Zubavichus, it was found that the lattice constants of the Nb3Sn phase in irradiated platelets increase up to 5.324 Å at 1×1022p/m2. The peak broadening at very high fluences is mainly attributed to microstrain effects. The enhancement of the lattice constants and microstrains for both the steady loss and Bragg peak regions are reported in Figure 71 as a function of the fluence.
Figure 71 Increase of the lattice constant (top) and microstrain (bottom) with fluence for both the steady loss and the Bragg peak regions. It should be noted that at 1 × 1022 p/m2 the value of the lattice constant for the sample in the Bragg peak region is lower than expected due to the presence of more than one A15 phases (explanation: see text).
For the higher fluences, i.e. 3 × 1021 p/m2 and 1 × 1022 p/m2, the Bragg peak platelets (samples
#2) are characterized by considerably larger microstrains. The inversion of this tendency for the lattice constant after 1 × 1022 p/m2 (a higher value for the platelets #1 with respect to #2) is explained taking into account the split of the peak (220) of sample #2, shown in Figure 72.
Indeed the available sample thickness (0.18 mm) is larger than the thickness of the total damage around the Bragg peak (calculated width: 0.05 to 0.1 mm, see Figure 16 in Chapter 1) thus the
“double” peak at high angles in sample #2 reflects the co-existence of two A15 phases with different degrees of order: the first one corresponds to a higher lattice constant at the Bragg peak (about 70% of the entire peak), the second one corresponds to the lattice constant in the region behind the Bragg peak (about 30%) being almost unchanged with respect to the state prior to irradiation reflecting the fact that after the Bragg peak there is no radiation damage.
It should be noticed that the increase of the microstrain induced in the platelets #1 (steady loss) is only 0.1% at the maximum fluence that is one order of magnitude higher than the highest fluence used for our proton irradiations on Nb3Sn wires (1.38× 1021 p/m2). At these fluences, as was explained in “Changes in Tc after irradiation” in Subsection 1.3.3, the effect of microstrains on the decrease of the critical temperature is negligible.
Figure 72 Comparison of the (220) peak between the pristine and the two platelets at the maximum fluence (𝟏𝟏×𝟏𝟏𝟎𝟎𝟐𝟐𝟐𝟐 p/m2). For sample #2 the irregular shape of the peak reflects the occurrence of two regions inside this sample only one of which being damaged.
The decrease of the Bragg Williams LRO order parameter, S, with fluence was estimated by Zubavichus studying the changes in the relative intensity of the (110) peak, normalized to the (210) peak, in analogy to the empirical method developed by the author (see Subsection 3.3.1).
As shown in Figure 73, the order parameter decrease with fluence and such decrease is stronger for the platelets #2 than for #1: as expected, the Bragg peak induced a higher disorder than the steady loss.
However the values of S found by means of X-ray powder diffraction (XRPD) are affected by a large uncertainty because the superlattice line (110) is very sensitivity to texture.
Figure 73 Decrease of the Bragg Williams LRO parameter, S, with fluence as estimated from the relative intensity of the (110) peak. The experimental pattern was measured by means of X-ray synchrotron diffraction (XRPD), i.e.
normal diffraction mode. In the Bragg peak region a stronger variation of S is shown.
Indeed, according to crystallographic simulations performed by Y. Zubavichus, for a fully ordered stoichiometric Nb3Sn, the relative intensity of the (110) peak with respect to the (210) peak is expected to be ~ 0.04 while the experimental value has been found in a larger range, i.e.
between 0.04 and 0.06. This fluctuation in the experimental intensity with respect to the theoretical one reveals that there are some additional factors affecting line intensities, such as preferred orientation or local inhomogeneities, which have not been taken into account leading to incorrect S values.
To improve the determination of S, a set of additional measurements near the absorption edge of Niobium, i.e. in the resonant diffraction mode, have been performed. By means of these measurements, the intensity of the (110) peak is increased nearly 3 times, allowing a better estimation of the order parameter.
The changes in the (110) intensity with fluence are shown in Figure 74 and the resulting S value in Figure 75.
Figure 74 Variation of the (110) intensity with fluence acquired in the resonant mode for the Bragg peak (dashed lines, samples #2) and the steady loss regions (continuous lines, samples #1).
In the resonant diffraction mode, the pristine sample is characterized by the maximum relative intensity of the (110) line, whereas the respective intensities for the proton-irradiated samples are systematically lower especially for those in the Bragg peak region.
The decrease of the order parameters S up to the maximum fluence of 1×1022 p/m2 for the platelets in the steady loss and at the Bragg peak is 3.1% and 14.2%, respectively.
Figure 75 Decrease of the Bragg Williams LRO parameter, S, with fluence as estimated from the relative intensity of the (110) peak. The experimental pattern was measured by means of resonant diffraction (REXD) that is texture independent allowing a better estimation of S. In the Bragg peak region a stronger variation of S is shown.